STRAIN GRADIENT PLASTICITY: THEORY AND EXPERIMENT plastic strain. A deformation theory of plasticity
Embed Size (px)
Transcript of STRAIN GRADIENT PLASTICITY: THEORY AND EXPERIMENT plastic strain. A deformation theory of plasticity
Acta metall, mater. Vol. 42, No. 2, pp. 475-487, 1994 0956-7151/94 $6.00 + 0.00 Printed in Great Britain. All rights reserved Copyright ~) 1994 Pergamon Press Ltd
STRAIN G R A D I E N T PLASTICITY: THEORY A N D E X P E R I M E N T
N. A. FLECK 1, G. M. M U L L E R 1, M. F. A S H B Y I and J. W. H U T C H I N S O N 2
ICambridge University Engineering Department, Trumpington Street, Cambridge CB2 1PZ, England and 2Division of Applied Sciences, Harvard University, Oxford Street, Cambridge, MA 02138, U.S.A.
(Received 5 March 1993," in revised form 24 June 1993)
Abstract--Dislocation theory is used to invoke a strain gradient theory of rate independent plasticity. Hardening is assumed to result from the accumulation of both randomly stored and geometrically necessary dislocations. The density of the geometrically necessary dislocations scales with the gradient of plastic strain. A deformation theory of plasticity is introduced to represent in a phenomenological manner the relative roles of strain hardening and strain gradient hardening. The theory is a non-linear generalization of Cosserat couple stress theory. Tension and torsion experiments on thin copper wires confirm the presence of strain gradient hardening. The experiments are interpreted in the light of the new theory.
1.1. Scale effects in plasticity
In this paper we develop a phenomenological plas- ticity law which accounts for a size dependence on strength. In conventional plasticity theory no length scale enters the constitutive law and no size effects are predicted. However, several observed plasticity phenomena display a size effect whereby the smaller is the size the stronger is the response. As examples: the indentation hardness of metals and ceramics increases as the size of the indenter is decreased ; the strengthening of metals by a given volume frac- tion of hard particles is greater for small particles than for large, for the same volume fraction of reinforcement, as is their rate of work hardening [2, 3]; and fine-grained metals are stronger than those with coarse grains . The effect becomes pronounced when the indent size, grain size or particle spacing lies below approximately 10 #m.
These effects may not all have the same expla- nation, but it is clear that all require a length scale for their interpretation. A natural way to include size effects in the constitutive law is to postulate that the yield stress depends both upon strain and strain gradient. We adopt this approach in the current paper, and provide evidence for the strengthening due to a strain gradient by experiments on the tension and torsion responses of thin copper wires. In tension the strain is uniform and no size dependence of strength is observed. In torsion, however, the thinner is the wire the greater is the gradient of strain for a given surface shear strain, and the stronger is the response.
Conventional plasticity theories, as we have said, possess no internal length scale. When the length scale associated with the deformation field is large, strain gradients are small and conventional theories
suffice. On the other hand, when the length scale associated with the deformation field is small com- pared to a material length scale explained below, it becomes necessary to include the strain gradient term in the constitutive law. The purpose of this paper is to present a plasticity theory which includes an internal material length scale, and to provide sup- porting experimental evidence. The underlying idea is that material hardening is controlled by the total density of dislocations, part of which derives from, and is directly proportional to, the gradient of strain. The distinction between dislocations stored during uniform straining and those necessitated by gradients of strain can be understood as follows.
When a plastic crystal is deformed, dislocations are generated, move, and are stored; the storage causes the material to work harden. Dislocations become stored for two reasons: they accumulate by trapping each other in a random way or they are required for compatible deformation of various parts of the crys- tal. The dislocations which trap each other randomly are referred to as statistically stored dislocations [5, 6]. As yet, there is no simple argument to estimate the density Ps of these dislocations, although it has been measured, as a function of strain, by numerous investigators.
Gradients of plastic shear result in the storage of geometrically necessary dislocations [5-8]. Plastic strain gradients appear either because of the geo- metry of loading or because the material itself is plastically inhomogeneous (containing non-deform- ing phases, for instance). As examples: in the plastic twisting of a cylinder or bending of a beam, the strain is finite at the surface but zero along the axis of twist or of bending [Fig. l(a, b)]; in the hardness test the strain is large immediately beneath the indenter but zero far from it; and in the plastic zone at the tip of
AMM 42,'~J 475
476 FLECK et al.:
- i - "
STRAIN GRADIENT PLASTICITY
"M \\\ I /I / \ R I i I
\ i'Ki I \ /
\ / \ I \
\ \ i /
I (c) (d)
- - y
(e> (f) Fig. 1. Plastic strain gradients are caused by the geometry of deformation (a, b), by local boundary
conditions (c, d) or by the microstructure itself (e, f).
a crack in an otherwise elastic medium steep gradients of plastic strain appear [Fig. l(c, d)]; in the defor- mation of plastic crystals containing hard, non- deforming particles local strain gradients are gener- ated between particles; and in the plastic deformation of polycrystals, the mismatch of slip at the bound-
aries of the grains can induce gradients of plastic strain there [Fig. l(e, f)]. In approximate terms, the magnitude of the plastic strain gradient is of the order of the average shear strain in the crystal divided by the local length scale ). of the deformation field. These strain gradients require, for compatibility reasons,
FLECK et al.: STRAIN GRADIENT PLASTICITY 477
the presence of geometrically necessary dislocations of density po, where 
47 pG ~ ~-~. (1.1)
Here, I' is the macroscopic plastic shear strain and b is the magnitude of the Burger's vector b. The geometrically necessary dislocations contribute to hardening and, in the limit that Pc ~> Ps, the macro- scopic shear yield stress r can be written approxi- mately as
T ~ C ' G b x / ~ (1.2)
where G is the shear modulus and C ' is a constant of order unity. In the torsion test, ,l is simply the radius of the cylinder; in bending it is the half thickness of the beam; in the hardness test it is related to the indent size; at the crack tip, to the plastic zone size; and in metals containing non-deforming particles ;t is related to the particle separation, approximately r/J~ where r is the radius and f is the volume fraction of the particles. In polycrystals one might expect it to be related to the grain size.
Direct support for the notion that geometrically necessary dislocations lead to enhanced hardening comes from the compression tests of Russell and Ashby , Brown and Stobbs  and many others. Here the plate-like 0' precipitates lead to the storage of geometrically necessary dislocations and the appearance of lattice curvature, in good agreement with equation (1.1); and the enhancement in flow stress scales as the square root of PG, as suggested by equation (1.2). The well known size effect in hardness has recently been given a quantitative interpretation in terms of geometrically necessary dislocations by Brown . Experimental data  confirm that fine grained metals work harden faster than coarse grained metals.
Conventional plasticity laws tacitly assume that PG ~ Ps and no length scale enters. Figure 2 shows a comparison of po and Ps as a function of shear strain y for a variety of microstructural length scales 2 for pure copper. The shaded band marked "Single Crystal" is the measured density Ps of statistically stored dislocations in single crystal copper, oriented for (initial) easy glide; it is derived from the measure- ments of Basinski and Basinski . There are three stages. In stage I, slip is on one system only, dis- locations trap as dipoles and dislocation storage is proportional to strain; in the second stage, slips are induced on secondary systems and the storage becomes proportional to the square of the strain; and in the final, third, stage, recovery mechanisms such as cross-slip deplete the dislocation population, reducing the rate of storage once more. In polycrys- tals, stages I and II are absent, and the storage rate is at first rapid, decreasing to an almost linear increase with strain (corresponding to parabolic hardening, a ocE °5) above a strain of a few percent, as
P (m -;
1.U 1U 2UU SHEAR STRAIN, "Y (%)
Fig. 2, The density of statistically stored dislocations Ps, and geometrically necessary dislocations Pc plotted against shear strain. The single crystal density Ps (shaded band) is taken from the experimental data of Basinski and Basinski ; that for polycrystals is inferred from stress-strain curves. The density PG is shown as a set of parallel lines for assumed values of microstructural length scale 2, using
shown in the shaded band labeled "Polycrystal". It is to be emphas